#------------------------------------------------------------------------------
#$Date: 2025-12-07 06:00:29 +0100 (Sun 07 de Dec de 2025) $
#$Revision: 304106 $
#$URL: svn://www.crystallography.net/cod/cif/7/71/98/7719862.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7719862
loop_
_publ_author_name
'Gragg, Madalyn R.'
'Iwanicki, Allana G.'
'Siegler, Maxime A.'
'McQueen, Tyrel M.'
_publ_section_title
;
 Hydroflux crystal growth of alkali tellurate oxide-hydroxides.
;
_journal_issue                   47
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              17638
_journal_page_last               17645
_journal_paper_doi               10.1039/d5dt01468a
_journal_volume                  54
_journal_year                    2025
_chemical_formula_moiety         'Cs2 Cu3 O10 Te2'
_chemical_formula_sum            'Cs2 Cu3 O10 Te2'
_chemical_formula_weight         871.64
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2019/3
_audit_update_record
;
2025-06-22 deposited with the CCDC.	2025-11-07 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 100.550(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.6630(2)
_cell_length_b                   14.6253(6)
_cell_length_c                   7.3375(3)
_cell_measurement_reflns_used    4357
_cell_measurement_temperature    213(2)
_cell_measurement_theta_max      33.1580
_cell_measurement_theta_min      2.7720
_cell_volume                     597.44(4)
_computing_cell_refinement       'CrysAlisPro 1.171.42.49 (Rigaku OD, 2022)'
_computing_data_collection       'CrysAlisPro 1.171.42.49 (Rigaku OD, 2022)'
_computing_data_reduction        'CrysAlisPro 1.171.42.49 (Rigaku OD, 2022)'
_computing_molecular_graphics    'SHELXTL v6.10 (Sheldrick, 2008)'
_computing_publication_material  'SHELXTL v6.10 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXS-2018/3 (Sheldrick, 2018)'
_diffrn_ambient_temperature      213(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Atlas'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_source         'SuperNova (Mo) X-ray Source'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0271
_diffrn_reflns_av_unetI/netI     0.0153
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            9086
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         33.000
_diffrn_reflns_theta_min         2.785
_exptl_absorpt_coefficient_mu    16.117
_exptl_absorpt_correction_T_max  0.765
_exptl_absorpt_correction_T_min  0.529
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.43.90 (Rigaku Oxford Diffraction, 2023)
Analytical numeric absorption correction using a multifaceted crystal
model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'pale blue'
_exptl_crystal_density_diffrn    4.845
_exptl_crystal_description       'small plate'
_exptl_crystal_F_000             762
_exptl_crystal_size_max          0.049
_exptl_crystal_size_mid          0.043
_exptl_crystal_size_min          0.018
_refine_diff_density_max         1.609
_refine_diff_density_min         -1.299
_refine_diff_density_rms         0.216
_refine_ls_extinction_coef       0.00124(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2019/2 (Sheldrick 2019)'
_refine_ls_goodness_of_fit_ref   1.231
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     110
_refine_ls_number_reflns         1166
_refine_ls_number_restraints     121
_refine_ls_restrained_S_all      1.248
_refine_ls_R_factor_all          0.0281
_refine_ls_R_factor_gt           0.0257
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0196P)²+8.1357P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0656
_refine_ls_wR_factor_ref         0.0668
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1090
_reflns_number_total             1166
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d5dt01468a2.cif
_cod_data_source_block           xs3345a
_cod_depositor_comments
'Adding full bibliography for 7719860--7719862.cif.'
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               7719862
_shelx_shelxl_version_number     2019/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_oxdiff_exptl_absorpt_empirical_full_min 0.813
_oxdiff_exptl_absorpt_empirical_full_max 1.327
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
- B-factor correction
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Te1 Te 0.500000 0.39500(2) 0.500000 0.00665(11) Uani 1 2 d S T P A .
Cu1 Cu 1.000000 0.30036(4) 0.500000 0.00965(14) Uani 1 2 d S T P A .
Cu2 Cu 1.000000 0.500000 0.500000 0.00763(16) Uani 1 4 d S T P A .
O1 O 0.4427(6) 0.500000 0.6605(5) 0.0084(6) Uani 1 2 d S T P A .
O2 O 0.5705(5) 0.30326(16) 0.3376(4) 0.0108(5) Uani 1 1 d . . . . .
O3 O 0.8382(4) 0.40113(16) 0.6098(4) 0.0086(4) Uani 1 1 d . . . . .
Cs1 Cs 0.8825(8) 0.3400(4) 1.0096(4) 0.0438(11) Uani 0.137(2) 1 d . U P A 1
Cs2 Cs 0.750000 0.250000 1.000000 0.043(2) Uani 0.081(3) 2 d S U P A 2
Cs3 Cs 0.9132(14) 0.4748(5) 1.0070(7) 0.058(2) Uani 0.0771(15) 1 d . U P A 3
Cs4 Cs 0.7940(6) 0.4066(3) 1.0162(3) 0.0529(11) Uani 0.1469(19) 1 d . U P A 4
Cs5 Cs 0.808(2) 0.2961(13) 1.0045(12) 0.046(2) Uani 0.054(2) 1 d . U P A 5
Cs6 Cs 0.674(7) 0.377(3) 1.011(4) 0.051(2) Uani 0.0142(13) 1 d . U P A 6
Cs7 Cs 1.000000 0.3328(16) 1.000000 0.043(3) Uani 0.038(3) 2 d S TU P A 7
Cs8 Cs 0.776(7) 0.500000 1.005(3) 0.057(3) Uani 0.024(2) 2 d S TU P A 8
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Te1 O2 89.23(16) . 2_656 ?
O2 Te1 O3 94.44(11) . 2_656 ?
O2 Te1 O3 89.33(11) 2_656 2_656 ?
O2 Te1 O3 89.33(11) . . ?
O2 Te1 O3 94.44(11) 2_656 . ?
O3 Te1 O3 174.70(14) 2_656 . ?
O2 Te1 O1 174.81(11) . . ?
O2 Te1 O1 95.65(11) 2_656 . ?
O3 Te1 O1 87.41(12) 2_656 . ?
O3 Te1 O1 88.52(13) . . ?
O2 Te1 O1 95.65(11) . 5_666 ?
O2 Te1 O1 174.81(11) 2_656 5_666 ?
O3 Te1 O1 88.52(12) 2_656 5_666 ?
O3 Te1 O1 87.41(12) . 5_666 ?
O1 Te1 O1 79.53(15) . 5_666 ?
O2 Te1 Cu1 44.61(8) . 7_656 ?
O2 Te1 Cu1 44.61(8) 2_656 7_656 ?
O3 Te1 Cu1 92.65(7) 2_656 7_656 ?
O3 Te1 Cu1 92.65(7) . 7_656 ?
O1 Te1 Cu1 140.23(8) . 7_656 ?
O1 Te1 Cu1 140.23(8) 5_666 7_656 ?
O2 Te1 Te1 135.39(8) . 5_666 ?
O2 Te1 Te1 135.39(8) 2_656 5_666 ?
O3 Te1 Te1 87.35(7) 2_656 5_666 ?
O3 Te1 Te1 87.35(7) . 5_666 ?
O1 Te1 Te1 39.77(8) . 5_666 ?
O1 Te1 Te1 39.77(8) 5_666 5_666 ?
Cu1 Te1 Te1 180.0 7_656 5_666 ?
O2 Te1 Cs6 122.7(7) . . ?
O2 Te1 Cs6 50.0(7) 2_656 . ?
O3 Te1 Cs6 118.9(6) 2_656 . ?
O3 Te1 Cs6 61.6(6) . . ?
O1 Te1 Cs6 60.1(7) . . ?
O1 Te1 Cs6 127.6(7) 5_666 . ?
Cu1 Te1 Cs6 85.8(7) 7_656 . ?
Te1 Te1 Cs6 94.2(7) 5_666 . ?
O2 Te1 Cs6 50.0(7) . 2_656 ?
O2 Te1 Cs6 122.7(7) 2_656 2_656 ?
O3 Te1 Cs6 61.6(6) 2_656 2_656 ?
O3 Te1 Cs6 118.9(6) . 2_656 ?
O1 Te1 Cs6 127.6(7) . 2_656 ?
O1 Te1 Cs6 60.1(7) 5_666 2_656 ?
Cu1 Te1 Cs6 85.8(7) 7_656 2_656 ?
Te1 Te1 Cs6 94.2(7) 5_666 2_656 ?
O2 Te1 Cs4 123.32(11) . . ?
O2 Te1 Cs4 60.87(11) 2_656 . ?
O3 Te1 Cs4 128.53(9) 2_656 . ?
O3 Te1 Cs4 51.17(9) . . ?
O1 Te1 Cs4 58.28(12) . . ?
O1 Te1 Cs4 117.28(12) 5_666 . ?
Cu1 Te1 Cs4 92.51(7) 7_656 . ?
Te1 Te1 Cs4 87.49(8) 5_666 . ?
O2 Te1 Cs4 60.87(11) . 2_656 ?
O2 Te1 Cs4 123.32(11) 2_656 2_656 ?
O3 Te1 Cs4 51.17(9) 2_656 2_656 ?
O3 Te1 Cs4 128.53(9) . 2_656 ?
O1 Te1 Cs4 117.28(12) . 2_656 ?
O1 Te1 Cs4 58.28(12) 5_666 2_656 ?
Cu1 Te1 Cs4 92.51(7) 7_656 2_656 ?
Te1 Te1 Cs4 87.49(7) 5_666 2_656 ?
O3 Cu1 O3 83.98(14) . 2_756 ?
O3 Cu1 O2 163.12(11) . 8 ?
O3 Cu1 O2 99.36(10) 2_756 8 ?
O3 Cu1 O2 99.36(10) . 7_656 ?
O3 Cu1 O2 163.12(11) 2_756 7_656 ?
O2 Cu1 O2 82.28(15) 8 7_656 ?
O3 Cu1 Te1 138.01(7) . 7_656 ?
O3 Cu1 Te1 138.01(7) 2_756 7_656 ?
O2 Cu1 Te1 41.14(7) 8 7_656 ?
O2 Cu1 Te1 41.14(7) 7_656 7_656 ?
O3 Cu1 Cu2 41.99(7) . . ?
O3 Cu1 Cu2 41.99(7) 2_756 . ?
O2 Cu1 Cu2 138.86(7) 8 . ?
O2 Cu1 Cu2 138.86(7) 7_656 . ?
Te1 Cu1 Cu2 180.0 7_656 . ?
O3 Cu1 Cs1 59.10(11) . 2_757 ?
O3 Cu1 Cs1 105.86(11) 2_756 2_757 ?
O2 Cu1 Cs1 134.07(11) 8 2_757 ?
O2 Cu1 Cs1 63.12(12) 7_656 2_757 ?
Te1 Cu1 Cs1 99.30(9) 7_656 2_757 ?
Cu2 Cu1 Cs1 80.70(9) . 2_757 ?
O3 Cu1 Cs1 105.86(11) . 1_554 ?
O3 Cu1 Cs1 59.10(11) 2_756 1_554 ?
O2 Cu1 Cs1 63.12(12) 8 1_554 ?
O2 Cu1 Cs1 134.07(11) 7_656 1_554 ?
Te1 Cu1 Cs1 99.30(9) 7_656 1_554 ?
Cu2 Cu1 Cs1 80.70(9) . 1_554 ?
Cs1 Cu1 Cs1 161.40(18) 2_757 1_554 ?
O3 Cu1 Cs5 71.3(3) . 2_757 ?
O3 Cu1 Cs5 110.3(2) 2_756 2_757 ?
O2 Cu1 Cs5 121.9(3) 8 2_757 ?
O2 Cu1 Cs5 56.3(3) 7_656 2_757 ?
Te1 Cu1 Cs5 89.0(3) 7_656 2_757 ?
Cu2 Cu1 Cs5 91.0(3) . 2_757 ?
Cs1 Cu1 Cs5 12.2(3) 2_757 2_757 ?
Cs1 Cu1 Cs5 169.4(3) 1_554 2_757 ?
O3 Cu1 Cs5 110.3(2) . 1_554 ?
O3 Cu1 Cs5 71.3(3) 2_756 1_554 ?
O2 Cu1 Cs5 56.3(3) 8 1_554 ?
O2 Cu1 Cs5 121.9(3) 7_656 1_554 ?
Te1 Cu1 Cs5 89.0(3) 7_656 1_554 ?
Cu2 Cu1 Cs5 91.0(3) . 1_554 ?
Cs1 Cu1 Cs5 169.4(3) 2_757 1_554 ?
Cs1 Cu1 Cs5 12.2(3) 1_554 1_554 ?
O3 Cu1 Cs7 54.4(3) . . ?
O3 Cu1 Cs7 113.1(3) 2_756 . ?
O2 Cu1 Cs7 136.0(3) 8 . ?
O2 Cu1 Cs7 58.2(4) 7_656 . ?
Te1 Cu1 Cs7 97.4(4) 7_656 . ?
Cu2 Cu1 Cs7 82.6(4) . . ?
O3 Cu1 Cs7 113.1(3) . 1_554 ?
O3 Cu1 Cs7 54.4(3) 2_756 1_554 ?
O2 Cu1 Cs7 58.2(4) 8 1_554 ?
O2 Cu1 Cs7 136.0(3) 7_656 1_554 ?
Te1 Cu1 Cs7 97.4(4) 7_656 1_554 ?
Cu2 Cu1 Cs7 82.6(4) . 1_554 ?
Cs1 Cu1 Cs7 160.2(3) 2_757 1_554 ?
Cs1 Cu1 Cs7 10.72(11) 1_554 1_554 ?
O3 Cu2 O3 85.06(14) 5_766 6_565 ?
O3 Cu2 O3 94.94(14) 5_766 2_756 ?
O3 Cu2 O3 180.0 6_565 2_756 ?
O3 Cu2 O3 180.0 5_766 . ?
O3 Cu2 O3 94.94(14) 6_565 . ?
O3 Cu2 O3 85.06(14) 2_756 . ?
O3 Cu2 Cu1 137.47(7) 5_766 . ?
O3 Cu2 Cu1 137.47(7) 6_565 . ?
O3 Cu2 Cu1 42.53(7) 2_756 . ?
O3 Cu2 Cu1 42.53(7) . . ?
O3 Cu2 Cu1 42.53(7) 5_766 5_766 ?
O3 Cu2 Cu1 42.53(7) 6_565 5_766 ?
O3 Cu2 Cu1 137.47(7) 2_756 5_766 ?
O3 Cu2 Cu1 137.47(7) . 5_766 ?
Cu1 Cu2 Cu1 180.0 . 5_766 ?
O3 Cu2 Cs3 110.57(14) 5_766 5_767 ?
O3 Cu2 Cs3 59.81(13) 6_565 5_767 ?
O3 Cu2 Cs3 120.19(13) 2_756 5_767 ?
O3 Cu2 Cs3 69.43(14) . 5_767 ?
Cu1 Cu2 Cs3 95.90(11) . 5_767 ?
Cu1 Cu2 Cs3 84.10(11) 5_766 5_767 ?
O3 Cu2 Cs3 69.43(14) 5_766 1_554 ?
O3 Cu2 Cs3 120.19(13) 6_565 1_554 ?
O3 Cu2 Cs3 59.81(13) 2_756 1_554 ?
O3 Cu2 Cs3 110.57(14) . 1_554 ?
Cu1 Cu2 Cs3 84.10(11) . 1_554 ?
Cu1 Cu2 Cs3 95.90(11) 5_766 1_554 ?
O3 Cu2 Cs3 59.81(13) 5_766 6_564 ?
O3 Cu2 Cs3 110.57(14) 6_565 6_564 ?
O3 Cu2 Cs3 69.43(14) 2_756 6_564 ?
O3 Cu2 Cs3 120.19(13) . 6_564 ?
Cu1 Cu2 Cs3 95.90(11) . 6_564 ?
Cu1 Cu2 Cs3 84.10(11) 5_766 6_564 ?
O3 Cu2 Cs3 120.19(13) 5_766 2_757 ?
O3 Cu2 Cs3 69.43(14) 6_565 2_757 ?
O3 Cu2 Cs3 110.57(14) 2_756 2_757 ?
O3 Cu2 Cs3 59.81(13) . 2_757 ?
Cu1 Cu2 Cs3 84.10(11) . 2_757 ?
Cu1 Cu2 Cs3 95.90(11) 5_766 2_757 ?
O3 Cu2 Cs8 108.0(4) 5_766 5_767 ?
O3 Cu2 Cs8 72.0(4) 6_565 5_767 ?
O3 Cu2 Cs8 108.0(4) 2_756 5_767 ?
O3 Cu2 Cs8 72.0(4) . 5_767 ?
Cu1 Cu2 Cs8 90.000(2) . 5_767 ?
Cu1 Cu2 Cs8 90.000(4) 5_766 5_767 ?
Cs3 Cu2 Cs8 13.6(5) 5_767 5_767 ?
Cs3 Cu2 Cs8 166.4(5) 1_554 5_767 ?
Cs3 Cu2 Cs8 166.4(6) 6_564 5_767 ?
Cs3 Cu2 Cs8 13.6(5) 2_757 5_767 ?
O3 Cu2 Cs8 72.0(4) 5_766 1_554 ?
O3 Cu2 Cs8 108.0(4) 6_565 1_554 ?
O3 Cu2 Cs8 72.0(4) 2_756 1_554 ?
O3 Cu2 Cs8 108.0(4) . 1_554 ?
Cu1 Cu2 Cs8 90.000(2) . 1_554 ?
Cu1 Cu2 Cs8 90.0 5_766 1_554 ?
Te1 O1 Te1 100.47(15) 5_666 . ?
Te1 O1 Cs8 111.6(5) 5_666 . ?
Te1 O1 Cs8 111.6(5) . . ?
Te1 O1 Cs8 129.05(13) 5_666 5_667 ?
Te1 O1 Cs8 129.05(13) . 5_667 ?
Te1 O1 Cs6 95.1(8) 5_666 5_667 ?
Te1 O1 Cs6 164.4(8) . 5_667 ?
Te1 O1 Cs6 164.4(8) 5_666 2_657 ?
Te1 O1 Cs6 95.1(8) . 2_657 ?
Te1 O1 Cs6 87.3(7) 5_666 6_565 ?
Te1 O1 Cs6 144.7(8) . 6_565 ?
Te1 O1 Cs6 144.7(8) 5_666 . ?
Te1 O1 Cs6 87.3(7) . . ?
Cs6 O1 Cs6 79.8(12) 5_667 . ?
Cs6 O1 Cs6 35.4(14) 2_657 . ?
Cs6 O1 Cs6 68.3(15) 6_565 . ?
Te1 O1 Cs4 103.98(10) 5_666 5_667 ?
Te1 O1 Cs4 153.05(13) . 5_667 ?
Te1 O1 Cs4 153.05(13) 5_666 2_657 ?
Te1 O1 Cs4 103.98(10) . 2_657 ?
Te1 O1 Cs4 90.48(11) 5_666 6_565 ?
Te1 O1 Cs4 130.51(16) . 6_565 ?
Te1 O1 Cs4 130.51(16) 5_666 . ?
Te1 O1 Cs4 90.48(11) . . ?
Cs4 O1 Cs4 82.23(14) 5_667 . ?
Cs4 O1 Cs4 60.81(12) 2_657 . ?
Cs4 O1 Cs4 49.31(17) 6_565 . ?
Te1 O2 Cu1 94.24(12) . 7_656 ?
Te1 O2 Cs6 111.9(9) . 1_554 ?
Cu1 O2 Cs6 153.6(9) 7_656 1_554 ?
Te1 O2 Cs6 100.0(9) . 2_656 ?
Cu1 O2 Cs6 133.7(8) 7_656 2_656 ?
Te1 O2 Cs2 124.06(12) . 2_656 ?
Cu1 O2 Cs2 98.21(10) 7_656 2_656 ?
Te1 O2 Cs2 149.79(12) . 1_554 ?
Cu1 O2 Cs2 115.76(10) 7_656 1_554 ?
Te1 O2 Cs5 110.7(4) . 2_656 ?
Cu1 O2 Cs5 106.4(3) 7_656 2_656 ?
Te1 O2 Cs5 136.9(4) . 8_454 ?
Cu1 O2 Cs5 89.7(3) 7_656 8_454 ?
Te1 O2 Cs5 135.9(4) . 1_554 ?
Cu1 O2 Cs5 128.6(4) 7_656 1_554 ?
Te1 O2 Cs5 162.6(3) . 7_656 ?
Cu1 O2 Cs5 103.0(4) 7_656 7_656 ?
Te1 O2 Cs7 159.6(2) . 7_656 ?
Cu1 O2 Cs7 88.8(3) 7_656 7_656 ?
Te1 O2 Cs1 148.87(15) . 8_454 ?
Cu1 O2 Cs1 83.02(11) 7_656 8_454 ?
Te1 O3 Cu2 111.30(12) . . ?
Te1 O3 Cu1 106.94(12) . . ?
Cu2 O3 Cu1 95.48(11) . . ?
Te1 O3 Cs7 119.02(15) . . ?
Cu2 O3 Cs7 123.5(3) . . ?
Cu1 O3 Cs7 93.3(3) . . ?
Te1 O3 Cs1 106.79(13) . . ?
Cu2 O3 Cs1 130.72(14) . . ?
Cu1 O3 Cs1 102.20(14) . . ?
Te1 O3 Cs4 99.01(11) . . ?
Cu2 O3 Cs4 120.82(13) . . ?
Cu1 O3 Cs4 123.06(14) . . ?
Te1 O3 Cs3 111.47(18) . . ?
Cu2 O3 Cs3 97.91(17) . . ?
Cu1 O3 Cs3 130.87(17) . . ?
Te1 O3 Cs1 131.89(14) . 2_757 ?
Cu2 O3 Cs1 112.68(14) . 2_757 ?
Cu1 O3 Cs1 87.36(12) . 2_757 ?
Cs1 O3 Cs1 25.76(17) . 2_757 ?
Te1 O3 Cs3 130.04(19) . 2_757 ?
Cu2 O3 Cs3 86.99(15) . 2_757 ?
Cu1 O3 Cs3 117.42(18) . 2_757 ?
Cs1 O3 Cs3 44.08(16) . 2_757 ?
Cs1 O3 Cs3 37.40(16) 2_757 2_757 ?
Te1 O3 Cs4 144.51(13) . 2_757 ?
Cu2 O3 Cs4 93.19(12) . 2_757 ?
Cu1 O3 Cs4 95.30(12) . 2_757 ?
Cs1 O3 Cs4 40.09(12) . 2_757 ?
Cs1 O3 Cs4 20.40(11) 2_757 2_757 ?
Te1 O3 Cs6 86.9(7) . . ?
Cu2 O3 Cs6 133.1(8) . . ?
Cu1 O3 Cs6 120.9(8) . . ?
Te1 O3 Cs5 97.9(2) . . ?
Cu2 O3 Cs5 143.5(3) . . ?
Cu1 O3 Cs5 96.5(3) . . ?
Cs1 Cs1 Cs1 118.77(19) 2_757 7_657 ?
Cs1 Cs1 O3 79.0(2) 2_757 . ?
Cs1 Cs1 O3 105.04(15) 7_657 . ?
Cs1 Cs1 O3 75.2(2) 2_757 2_757 ?
Cs1 Cs1 O3 117.62(16) 7_657 2_757 ?
O3 Cs1 O3 136.83(19) . 2_757 ?
Cs1 Cs1 O2 83.2(2) 2_757 8_556 ?
Cs1 Cs1 O2 63.99(15) 7_657 8_556 ?
O3 Cs1 O2 150.70(19) . 8_556 ?
O3 Cs1 O2 57.77(8) 2_757 8_556 ?
Cs1 Cs1 O2 138.0(3) 2_757 1_556 ?
Cs1 Cs1 O2 64.00(13) 7_657 1_556 ?
O3 Cs1 O2 142.90(17) . 1_556 ?
O3 Cs1 O2 68.80(9) 2_757 1_556 ?
O2 Cs1 O2 59.60(8) 8_556 1_556 ?
Cs1 Cs1 O2 123.6(3) 2_757 2_656 ?
Cs1 Cs1 O2 60.95(13) 7_657 2_656 ?
O3 Cs1 O2 52.30(8) . 2_656 ?
O3 Cs1 O2 160.33(18) 2_757 2_656 ?
O2 Cs1 O2 124.95(16) 8_556 2_656 ?
O2 Cs1 O2 95.30(13) 1_556 2_656 ?
Cs1 Cs1 O2 72.92(18) 2_757 7_656 ?
Cs1 Cs1 O2 61.79(15) 7_657 7_656 ?
O3 Cs1 O2 56.79(8) . 7_656 ?
O3 Cs1 O2 140.63(18) 2_757 7_656 ?
O2 Cs1 O2 95.76(17) 8_556 7_656 ?
O2 Cs1 O2 125.79(16) 1_556 7_656 ?
O2 Cs1 O2 58.07(8) 2_656 7_656 ?
Cs1 Cs1 Cu1 95.6(2) 2_757 1_556 ?
Cs1 Cs1 Cu1 84.56(12) 7_657 1_556 ?
O3 Cs1 Cu1 170.35(18) . 1_556 ?
O3 Cs1 Cu1 33.54(5) 2_757 1_556 ?
O2 Cs1 Cu1 33.86(5) 8_556 1_556 ?
O2 Cs1 Cu1 42.52(6) 1_556 1_556 ?
O2 Cs1 Cu1 136.16(14) 2_656 1_556 ?
O2 Cs1 Cu1 129.57(16) 7_656 1_556 ?
Cs1 Cs1 Cs1 43.22(12) 2_757 8 ?
Cs1 Cs1 Cs1 76.4(3) 7_657 8 ?
O3 Cs1 Cs1 97.57(9) . 8 ?
O3 Cs1 Cs1 86.74(8) 2_757 8 ?
O2 Cs1 Cs1 54.24(13) 8_556 8 ?
O2 Cs1 Cs1 112.43(16) 1_556 8 ?
O2 Cs1 Cs1 110.72(16) 2_656 8 ?
O2 Cs1 Cs1 54.09(11) 7_656 8 ?
Cu1 Cs1 Cs1 83.61(9) 1_556 8 ?
Cs1 Cs1 Cs1 136.78(12) 2_757 8_455 ?
Cs1 Cs1 Cs1 18.00(15) 7_657 8_455 ?
O3 Cs1 Cs1 105.66(9) . 8_455 ?
O3 Cs1 Cs1 116.89(10) 2_757 8_455 ?
O2 Cs1 Cs1 72.49(15) 8_556 8_455 ?
O2 Cs1 Cs1 52.81(6) 1_556 8_455 ?
O2 Cs1 Cs1 54.93(6) 2_656 8_455 ?
O2 Cs1 Cs1 74.59(14) 7_656 8_455 ?
Cu1 Cs1 Cs1 83.76(9) 1_556 8_455 ?
Cs1 Cs1 Cs1 94.2(2) 8 8_455 ?
Cs1 Cs1 Cu1 64.3(2) 2_757 . ?
Cs1 Cs1 Cu1 89.80(15) 7_657 . ?
O3 Cs1 Cu1 29.31(6) . . ?
O3 Cs1 Cu1 138.75(15) 2_757 . ?
O2 Cs1 Cu1 121.40(16) 8_556 . ?
O2 Cs1 Cu1 151.08(15) 1_556 . ?
O2 Cs1 Cu1 59.34(7) 2_656 . ?
O2 Cs1 Cu1 30.54(5) 7_656 . ?
Cu1 Cs1 Cu1 153.14(15) 1_556 . ?
Cs1 Cs1 Cu1 69.55(6) 8 . ?
Cs1 Cs1 Cu1 98.63(10) 8_455 . ?
O2 Cs2 O2 180.0 8_556 2_656 ?
O2 Cs2 O2 112.89(7) 8_556 7_656 ?
O2 Cs2 O2 67.11(7) 2_656 7_656 ?
O2 Cs2 O2 67.11(7) 8_556 1_556 ?
O2 Cs2 O2 112.89(7) 2_656 1_556 ?
O2 Cs2 O2 180.0 7_656 1_556 ?
Cs2 Cs2 O3 74.04(4) 2_757 . ?
Cs2 Cs2 O3 105.96(4) 2_657 . ?
O2 Cs2 O3 131.77(7) 8_556 . ?
O2 Cs2 O3 48.23(7) 2_656 . ?
O2 Cs2 O3 52.80(6) 7_656 . ?
O2 Cs2 O3 127.20(6) 1_556 . ?
O2 Cs2 O3 48.23(7) 8_556 7_657 ?
O2 Cs2 O3 131.77(7) 2_656 7_657 ?
O2 Cs2 O3 127.20(6) 7_656 7_657 ?
O2 Cs2 O3 52.80(6) 1_556 7_657 ?
O3 Cs2 O3 180.0 . 7_657 ?
O2 Cs2 Cu1 147.98(5) 8_556 7_656 ?
O2 Cs2 Cu1 32.02(5) 2_656 7_656 ?
O2 Cs2 Cu1 41.76(5) 7_656 7_656 ?
O2 Cs2 Cu1 138.24(6) 1_556 7_656 ?
O3 Cs2 Cu1 56.27(4) . 7_656 ?
O3 Cs2 Cu1 123.73(4) 7_657 7_656 ?
O2 Cs2 Cu1 32.02(5) 8_556 1_556 ?
O2 Cs2 Cu1 147.98(5) 2_656 1_556 ?
O2 Cs2 Cu1 138.24(5) 7_656 1_556 ?
O2 Cs2 Cu1 41.76(6) 1_556 1_556 ?
O3 Cs2 Cu1 123.73(4) . 1_556 ?
O3 Cs2 Cu1 56.27(4) 7_657 1_556 ?
Cu1 Cs2 Cu1 180.0 7_656 1_556 ?
O2 Cs2 Cu1 57.89(5) 8_556 7_657 ?
O2 Cs2 Cu1 122.11(5) 2_656 7_657 ?
O2 Cs2 Cu1 154.65(5) 7_656 7_657 ?
O2 Cs2 Cu1 25.35(5) 1_556 7_657 ?
O3 Cs2 Cu1 152.06(4) . 7_657 ?
O3 Cs2 Cu1 27.94(4) 7_657 7_657 ?
Cu1 Cs2 Cu1 133.366(8) 7_656 7_657 ?
Cu1 Cs2 Cu1 46.634(8) 1_556 7_657 ?
Cs2 Cs2 Cu1 60.444(3) 2_757 . ?
Cs2 Cs2 Cu1 119.556(3) 2_657 . ?
O2 Cs2 Cu1 122.11(5) 8_556 . ?
O2 Cs2 Cu1 57.89(5) 2_656 . ?
O2 Cs2 Cu1 25.35(5) 7_656 . ?
O2 Cs2 Cu1 154.65(5) 1_556 . ?
O3 Cs2 Cu1 27.94(4) . . ?
O3 Cs2 Cu1 152.06(4) 7_657 . ?
Cu1 Cs2 Cu1 46.634(7) 7_656 . ?
Cu1 Cs2 Cu1 133.366(8) 1_556 . ?
Cu1 Cs2 Cu1 180.0 7_657 . ?
Cs3 Cs3 O3 110.61(13) 6_565 . ?
Cs3 Cs3 O3 82.5(5) 2_757 . ?
Cs3 Cs3 O3 95.9(5) 5_767 . ?
O3 Cs3 O3 134.6(2) . 2_757 ?
Cs3 Cs3 O1 83.69(11) 6_565 . ?
Cs3 Cs3 O1 125.3(6) 2_757 . ?
Cs3 Cs3 O1 113.7(5) 5_767 . ?
O3 Cs3 O1 50.51(10) . . ?
O3 Cs3 O1 153.3(3) 2_757 . ?
O3 Cs3 O3 52.93(12) . 6_565 ?
O3 Cs3 O3 158.5(3) 2_757 6_565 ?
O1 Cs3 O3 48.10(10) . 6_565 ?
O3 Cs3 O3 158.8(3) . 5_767 ?
O3 Cs3 O3 52.35(11) 2_757 5_767 ?
O1 Cs3 O3 135.7(2) . 5_767 ?
O3 Cs3 O3 113.0(2) 6_565 5_767 ?
O3 Cs3 O1 135.4(3) . 5_667 ?
O3 Cs3 O1 67.88(13) 2_757 5_667 ?
O1 Cs3 O1 92.2(2) . 5_667 ?
O3 Cs3 O1 123.5(2) 6_565 5_667 ?
O3 Cs3 O1 64.50(12) 5_767 5_667 ?
O3 Cs3 Cu2 165.3(2) . 1_556 ?
O3 Cs3 Cu2 33.20(7) 2_757 1_556 ?
O1 Cs3 Cu2 134.3(2) . 1_556 ?
O3 Cs3 Cu2 141.8(2) 6_565 1_556 ?
O3 Cs3 Cu2 32.45(6) 5_767 1_556 ?
O1 Cs3 Cu2 42.76(9) 5_667 1_556 ?
Cs3 Cs3 Cu2 84.53(10) 6_565 . ?
Cs3 Cs3 Cu2 66.5(5) 2_757 . ?
Cs3 Cs3 Cu2 67.8(4) 5_767 . ?
O3 Cs3 Cu2 30.25(7) . . ?
O3 Cs3 Cu2 142.3(2) 2_757 . ?
O1 Cs3 Cu2 58.78(10) . . ?
O3 Cs3 Cu2 30.55(6) 6_565 . ?
O3 Cs3 Cu2 129.4(2) 5_767 . ?
O1 Cs3 Cu2 149.8(2) 5_667 . ?
Cu2 Cs3 Cu2 161.2(2) 1_556 . ?
Cs3 Cs3 Te1 106.21(9) 6_565 . ?
Cs3 Cs3 Te1 107.8(6) 2_757 . ?
Cs3 Cs3 Te1 114.3(5) 5_767 . ?
O3 Cs3 Te1 25.56(7) . . ?
O3 Cs3 Te1 142.9(2) 2_757 . ?
O1 Cs3 Te1 28.08(6) . . ?
O3 Cs3 Te1 54.79(8) 6_565 . ?
O3 Cs3 Te1 163.2(2) 5_767 . ?
O1 Cs3 Te1 110.7(2) 5_667 . ?
Cu2 Cs3 Te1 151.5(2) 1_556 . ?
Cu2 Cs3 Te1 47.02(6) . . ?
Cs4 Cs4 O3 69.21(12) 2_757 . ?
Cs4 Cs4 O3 91.50(10) 6_565 . ?
O3 Cs4 O3 134.36(12) . 2_757 ?
O3 Cs4 O1 148.28(17) . 5_667 ?
O3 Cs4 O1 70.48(10) 2_757 5_667 ?
O3 Cs4 O2 144.47(16) . 1_556 ?
O3 Cs4 O2 68.68(9) 2_757 1_556 ?
O1 Cs4 O2 52.74(7) 5_667 1_556 ?
Cs4 Cs4 O1 112.51(14) 2_757 . ?
Cs4 Cs4 O1 65.35(9) 6_565 . ?
O3 Cs4 O1 51.42(8) . . ?
O3 Cs4 O1 156.80(18) 2_757 . ?
O1 Cs4 O1 97.77(14) 5_667 . ?
O2 Cs4 O1 120.79(13) 1_556 . ?
O3 Cs4 Cs4 101.13(12) . 2_657 ?
O3 Cs4 Cs4 124.41(13) 2_757 2_657 ?
O1 Cs4 Cs4 60.24(10) 5_667 2_657 ?
O2 Cs4 Cs4 61.90(10) 1_556 2_657 ?
O1 Cs4 Cs4 58.95(9) . 2_657 ?
O3 Cs4 O2 51.70(8) . 2_656 ?
O3 Cs4 O2 151.83(18) 2_757 2_656 ?
O1 Cs4 O2 118.53(13) 5_667 2_656 ?
O2 Cs4 O2 94.93(13) 1_556 2_656 ?
O1 Cs4 O2 51.35(7) . 2_656 ?
O3 Cs4 Cs4 77.65(10) . 5_767 ?
O3 Cs4 Cs4 75.15(11) 2_757 5_767 ?
O1 Cs4 Cs4 95.01(17) 5_667 5_767 ?
O2 Cs4 Cs4 137.62(14) 1_556 5_767 ?
O1 Cs4 Cs4 86.43(14) . 5_767 ?
O2 Cs4 Cs4 126.77(12) 2_656 5_767 ?
O3 Cs4 Cu2 149.72(14) . 1_556 ?
O3 Cs4 Cu2 31.19(5) 2_757 1_556 ?
O1 Cs4 Cu2 42.01(7) 5_667 1_556 ?
O2 Cs4 Cu2 65.21(6) 1_556 1_556 ?
O1 Cs4 Cu2 129.39(15) . 1_556 ?
O2 Cs4 Cu2 157.87(11) 2_656 1_556 ?
Cs4 Cs4 Te1 99.01(13) 2_757 . ?
Cs4 Cs4 Te1 92.51(7) 6_565 . ?
O3 Cs4 Te1 29.82(5) . . ?
O3 Cs4 Te1 163.78(13) 2_757 . ?
O1 Cs4 Te1 125.26(13) 5_667 . ?
O2 Cs4 Te1 122.55(12) 1_556 . ?
O1 Cs4 Te1 31.24(4) . . ?
Cs4 Cs4 Te1 71.33(9) 2_657 . ?
O2 Cs4 Te1 29.30(5) 2_656 . ?
Cs4 Cs4 Te1 97.82(10) 5_767 . ?
Cu2 Cs4 Te1 160.38(15) 1_556 . ?
O2 Cs5 O2 151.0(7) 2_656 8_556 ?
O2 Cs5 O2 108.9(4) 2_656 1_556 ?
O2 Cs5 O2 65.3(2) 8_556 1_556 ?
O2 Cs5 O2 64.3(2) 2_656 7_656 ?
O2 Cs5 O2 106.5(4) 8_556 7_656 ?
O2 Cs5 O2 151.6(7) 1_556 7_656 ?
O2 Cs5 Cs5 121.6(3) 2_656 8 ?
O2 Cs5 Cs5 58.5(3) 8_556 8 ?
O2 Cs5 Cs5 123.7(3) 1_556 8 ?
O2 Cs5 Cs5 57.4(3) 7_656 8 ?
O2 Cs5 Cs5 60.43(19) 2_656 8_455 ?
O2 Cs5 Cs5 96.0(7) 8_556 8_455 ?
O2 Cs5 Cs5 58.36(17) 1_556 8_455 ?
O2 Cs5 Cs5 97.7(7) 7_656 8_455 ?
Cs5 Cs5 O3 118.2(8) 7_657 . ?
Cs5 Cs5 O3 76.3(4) 2_757 . ?
O2 Cs5 O3 52.63(17) 2_656 . ?
O2 Cs5 O3 147.4(4) 8_556 . ?
O2 Cs5 O3 143.1(5) 1_556 . ?
O2 Cs5 O3 56.75(17) 7_656 . ?
Cs5 Cs5 O3 90.5(3) 8 . ?
Cs5 Cs5 O3 113.00(18) 8_455 . ?
O2 Cs5 Cs5 54.6(3) 2_656 2_657 ?
O2 Cs5 Cs5 111.2(4) 8_556 2_657 ?
O2 Cs5 Cs5 54.4(3) 1_556 2_657 ?
O2 Cs5 Cs5 110.9(4) 7_656 2_657 ?
O3 Cs5 Cs5 101.3(3) . 2_657 ?
O2 Cs5 O3 151.4(6) 2_656 2_757 ?
O2 Cs5 O3 55.19(18) 8_556 2_757 ?
O2 Cs5 O3 66.6(2) 1_556 2_757 ?
O2 Cs5 O3 133.1(4) 7_656 2_757 ?
O3 Cs5 O3 112.9(6) . 2_757 ?
O2 Cs5 Cu1 152.3(4) 2_656 1_556 ?
O2 Cs5 Cu1 33.99(10) 8_556 1_556 ?
O2 Cs5 Cu1 43.45(13) 1_556 1_556 ?
O2 Cs5 Cu1 139.4(4) 7_656 1_556 ?
O3 Cs5 Cu1 145.2(6) . 1_556 ?
O3 Cs5 Cu1 32.37(10) 2_757 1_556 ?
O2 Cs6 O2 118.6(16) 1_556 2_656 ?
O2 Cs6 O1 57.3(6) 1_556 5_667 ?
O2 Cs6 O1 138.8(14) 2_656 5_667 ?
Cs6 Cs6 O1 71.2(12) 2_657 . ?
O2 Cs6 O1 141.8(14) 1_556 . ?
O2 Cs6 O1 56.0(5) 2_656 . ?
O1 Cs6 O1 100.2(12) 5_667 . ?
Cs6 Cs6 O3 112.2(17) 2_657 . ?
O2 Cs6 O3 163.3(17) 1_556 . ?
O2 Cs6 O3 53.9(5) 2_656 . ?
O1 Cs6 O3 139.0(15) 5_667 . ?
O1 Cs6 O3 50.2(5) . . ?
O2 Cs6 O3 67.7(6) 1_556 2_757 ?
O2 Cs6 O3 155.2(14) 2_656 2_757 ?
O1 Cs6 O3 65.7(6) 5_667 2_757 ?
O1 Cs6 O3 135.4(15) . 2_757 ?
O3 Cs6 O3 112.6(12) . 2_757 ?
O2 Cs6 Cs6 112.6(9) 1_556 6_565 ?
O2 Cs6 Cs6 111.8(9) 2_656 6_565 ?
O1 Cs6 Cs6 55.4(8) 5_667 6_565 ?
O1 Cs6 Cs6 55.9(7) . 6_565 ?
O3 Cs6 Cs6 83.7(8) . 6_565 ?
O3 Cs6 Cs6 84.2(7) 2_757 6_565 ?
Cs6 Cs6 Te1 80.8(15) 2_657 . ?
O2 Cs6 Te1 147.1(15) 1_556 . ?
O2 Cs6 Te1 30.1(3) 2_656 . ?
O1 Cs6 Te1 132.3(12) 5_667 . ?
O1 Cs6 Te1 32.6(2) . . ?
O3 Cs6 Te1 31.5(2) . . ?
O3 Cs6 Te1 143.8(12) 2_757 . ?
Cs6 Cs6 Te1 85.8(7) 6_565 . ?
O2 Cs6 Cs6 113.7(12) 1_556 2_757 ?
O2 Cs6 Cs6 106.3(11) 2_656 2_757 ?
O1 Cs6 Cs6 112.2(10) 5_667 2_757 ?
O1 Cs6 Cs6 103.1(10) . 2_757 ?
O3 Cs6 Cs6 60.9(8) . 2_757 ?
O3 Cs6 Cs6 53.1(7) 2_757 2_757 ?
Te1 Cs6 Cs6 92.2(10) . 2_757 ?
O2 Cs6 Cs6 75.3(12) 1_556 7_657 ?
O2 Cs6 Cs6 71.2(11) 2_656 7_657 ?
O1 Cs6 Cs6 131.6(14) 5_667 7_657 ?
O1 Cs6 Cs6 125.0(12) . 7_657 ?
O3 Cs6 Cs6 88.0(11) . 7_657 ?
O3 Cs6 Cs6 88.9(11) 2_757 7_657 ?
Te1 Cs6 Cs6 92.8(10) . 7_657 ?
O2 Cs6 Cu1 40.0(4) 1_556 1_556 ?
O2 Cs6 Cu1 141.5(15) 2_656 1_556 ?
O1 Cs6 Cu1 65.9(5) 5_667 1_556 ?
O1 Cs6 Cu1 162.5(14) . 1_556 ?
O3 Cs6 Cu1 134.3(12) . 1_556 ?
O3 Cs6 Cu1 30.5(2) 2_757 1_556 ?
Te1 Cs6 Cu1 161.4(12) . 1_556 ?
O3 Cs7 O3 141.2(8) . 2_757 ?
O3 Cs7 O2 59.25(11) . 7_656 ?
O3 Cs7 O2 158.6(7) 2_757 7_656 ?
O3 Cs7 O2 158.6(7) . 8_556 ?
O3 Cs7 O2 59.25(11) 2_757 8_556 ?
O2 Cs7 O2 101.5(7) 7_656 8_556 ?
O3 Cs7 Cu1 32.35(6) . . ?
O3 Cs7 Cu1 158.4(4) 2_757 . ?
O2 Cs7 Cu1 32.94(6) 7_656 . ?
O2 Cs7 Cu1 132.6(7) 8_556 . ?
O3 Cs7 Cu1 158.4(4) . 1_556 ?
O3 Cs7 Cu1 32.35(6) 2_757 1_556 ?
O2 Cs7 Cu1 132.6(7) 7_656 1_556 ?
O2 Cs7 Cu1 32.94(6) 8_556 1_556 ?
Cu1 Cs7 Cu1 165.3(7) . 1_556 ?
O3 Cs7 O2 47.89(6) . 2_656 ?
O3 Cs7 O2 138.4(2) 2_757 2_656 ?
O2 Cs7 O2 55.42(13) 7_656 2_656 ?
O2 Cs7 O2 114.9(4) 8_556 2_656 ?
Cu1 Cs7 O2 58.81(6) . 2_656 ?
Cu1 Cs7 O2 119.21(15) 1_556 2_656 ?
O3 Cs7 O2 138.4(2) . 1_656 ?
O3 Cs7 O2 47.89(6) 2_757 1_656 ?
O2 Cs7 O2 114.9(4) 7_656 1_656 ?
O2 Cs7 O2 55.42(13) 8_556 1_656 ?
Cu1 Cs7 O2 119.21(15) . 1_656 ?
Cu1 Cs7 O2 58.81(6) 1_556 1_656 ?
O2 Cs7 O2 166.7(7) 2_656 1_656 ?
O3 Cs7 Cs7 96.70(10) . 7_657 ?
O3 Cs7 Cs7 108.34(16) 2_757 7_657 ?
O2 Cs7 Cs7 66.6(5) 7_656 7_657 ?
O2 Cs7 Cs7 64.9(5) 8_556 7_657 ?
Cu1 Cs7 Cs7 93.1(4) . 7_657 ?
Cu1 Cs7 Cs7 77.2(2) 1_556 7_657 ?
O2 Cs7 Cs7 49.99(4) 2_656 7_657 ?
O2 Cs7 Cs7 119.5(6) 1_656 7_657 ?
O3 Cs7 Cs7 108.34(16) . 7_757 ?
O3 Cs7 Cs7 96.70(10) 2_757 7_757 ?
O2 Cs7 Cs7 64.9(5) 7_656 7_757 ?
O2 Cs7 Cs7 66.6(5) 8_556 7_757 ?
Cu1 Cs7 Cs7 77.2(2) . 7_757 ?
Cu1 Cs7 Cs7 93.1(4) 1_556 7_757 ?
O2 Cs7 Cs7 119.5(6) 2_656 7_757 ?
O2 Cs7 Cs7 49.99(4) 1_656 7_757 ?
O3 Cs7 O2 122.51(16) . 1_556 ?
O3 Cs7 O2 62.48(7) 2_757 1_556 ?
O2 Cs7 O2 115.9(4) 7_656 1_556 ?
O2 Cs7 O2 54.47(12) 8_556 1_556 ?
Cu1 Cs7 O2 138.4(2) . 1_556 ?
Cu1 Cs7 O2 39.00(5) 1_556 1_556 ?
O2 Cs7 O2 80.76(9) 2_656 1_556 ?
O2 Cs7 O2 97.71(11) 1_656 1_556 ?
O3 Cs7 O2 62.48(7) . 2_756 ?
O3 Cs7 O2 122.51(16) 2_757 2_756 ?
O2 Cs7 O2 54.47(12) 7_656 2_756 ?
O2 Cs7 O2 115.9(4) 8_556 2_756 ?
Cu1 Cs7 O2 39.00(5) . 2_756 ?
Cu1 Cs7 O2 138.4(2) 1_556 2_756 ?
O2 Cs7 O2 97.71(11) 2_656 2_756 ?
O2 Cs7 O2 80.76(9) 1_656 2_756 ?
O2 Cs7 O2 167.0(7) 1_556 2_756 ?
Cs8 Cs8 O1 118.5(15) 5_767 . ?
O1 Cs8 O1 115.1(14) . 5_667 ?
O1 Cs8 Cs8 58.9(9) . 5_667 ?
O1 Cs8 Cs8 56.2(10) 5_667 5_667 ?
O1 Cs8 O3 52.2(4) . 6_565 ?
O1 Cs8 O3 148.9(8) 5_667 6_565 ?
Cs8 Cs8 O3 73.3(11) 5_767 . ?
O1 Cs8 O3 52.2(4) . . ?
O1 Cs8 O3 148.9(8) 5_667 . ?
Cs8 Cs8 O3 104.3(11) 5_667 . ?
O3 Cs8 O3 51.8(4) 6_565 . ?
O1 Cs8 O3 155.94(18) . 5_767 ?
O1 Cs8 O3 68.1(5) 5_667 5_767 ?
O3 Cs8 O3 111.8(8) 6_565 5_767 ?
O3 Cs8 O3 136.6(13) . 5_767 ?
O1 Cs8 O3 155.94(18) . 2_757 ?
O1 Cs8 O3 68.1(5) 5_667 2_757 ?
O3 Cs8 O3 136.6(13) 6_565 2_757 ?
O3 Cs8 O3 111.8(8) . 2_757 ?
O3 Cs8 O3 48.1(4) 5_767 2_757 ?
O1 Cs8 Cu2 159.6(14) . 1_556 ?
O1 Cs8 Cu2 44.5(3) 5_667 1_556 ?
O3 Cs8 Cu2 143.5(9) 6_565 1_556 ?
O3 Cs8 Cu2 143.5(9) . 1_556 ?
O3 Cs8 Cu2 31.7(2) 5_767 1_556 ?
O3 Cs8 Cu2 31.7(2) 2_757 1_556 ?
O1 Cs8 Te1 27.32(19) . 5_666 ?
O1 Cs8 Te1 127.7(11) 5_667 5_666 ?
O3 Cs8 Te1 28.4(2) 6_565 5_666 ?
O3 Cs8 Te1 56.7(4) . 5_666 ?
O3 Cs8 Te1 130.8(4) 5_767 5_666 ?
O3 Cs8 Te1 164.1(12) 2_757 5_666 ?
Cu2 Cs8 Te1 157.3(2) 1_556 5_666 ?
Cs8 Cs8 Te1 101.3(12) 5_767 . ?
O1 Cs8 Te1 27.32(19) . . ?
O1 Cs8 Te1 127.7(11) 5_667 . ?
Cs8 Cs8 Te1 76.2(9) 5_667 . ?
O3 Cs8 Te1 56.7(4) 6_565 . ?
O3 Cs8 Te1 28.4(2) . . ?
O3 Cs8 Te1 164.1(12) 5_767 . ?
O3 Cs8 Te1 130.8(4) 2_757 . ?
Cu2 Cs8 Te1 157.3(2) 1_556 . ?
Te1 Cs8 Te1 44.6(3) 5_666 . ?
Cs8 Cs8 Cu2 60.4(11) 5_767 . ?
O1 Cs8 Cu2 58.0(5) . . ?
O1 Cs8 Cu2 173.1(12) 5_667 . ?
Cs8 Cs8 Cu2 116.9(11) 5_667 . ?
O3 Cs8 Cu2 28.0(3) 6_565 . ?
O3 Cs8 Cu2 28.0(3) . . ?
O3 Cs8 Cu2 118.1(10) 5_767 . ?
O3 Cs8 Cu2 118.1(10) 2_757 . ?
Cu2 Cs8 Cu2 142.4(12) 1_556 . ?
Te1 Cs8 Cu2 46.4(3) 5_666 . ?
Te1 Cs8 Cu2 46.4(3) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Te1 O2 1.885(3) . ?
Te1 O2 1.885(3) 2_656 ?
Te1 O3 1.939(2) 2_656 ?
Te1 O3 1.939(2) . ?
Te1 O1 1.998(2) . ?
Te1 O1 1.998(2) 5_666 ?
Te1 Cu1 2.8571(6) 7_656 ?
Te1 Te1 3.0712(6) 5_666 ?
Te1 Cs6 3.71(3) . ?
Te1 Cs6 3.71(3) 2_656 ?
Te1 Cs4 3.852(3) . ?
Te1 Cs4 3.852(3) 2_656 ?
Cu1 O3 1.983(2) . ?
Cu1 O3 1.983(2) 2_756 ?
Cu1 O2 2.012(3) 8 ?
Cu1 O2 2.012(3) 7_656 ?
Cu1 Cu2 2.9198(6) . ?
Cu1 Cs1 3.585(3) 2_757 ?
Cu1 Cs1 3.585(3) 1_554 ?
Cu1 Cs5 3.599(9) 2_757 ?
Cu1 Cs5 3.599(9) 1_554 ?
Cu1 Cs7 3.699(3) . ?
Cu1 Cs7 3.699(3) 1_554 ?
Cu2 O3 1.962(2) 5_766 ?
Cu2 O3 1.962(2) 6_565 ?
Cu2 O3 1.962(2) 2_756 ?
Cu2 O3 1.962(2) . ?
Cu2 Cs3 3.579(5) 5_767 ?
Cu2 Cs3 3.579(5) 1_554 ?
Cu2 Cs3 3.579(5) 6_564 ?
Cu2 Cs3 3.579(5) 2_757 ?
Cu2 Cs8 3.62(2) 5_767 ?
Cu2 Cs8 3.62(2) 1_554 ?
O1 Cs8 2.86(3) . ?
O1 Cs8 2.95(3) 5_667 ?
O1 Cs6 3.18(3) 5_667 ?
O1 Cs6 3.18(3) 2_657 ?
O1 Cs6 3.22(3) 6_565 ?
O1 Cs6 3.22(3) . ?
O1 Cs4 3.234(5) 5_667 ?
O1 Cs4 3.234(5) 2_657 ?
O1 Cs4 3.276(5) 6_565 ?
O1 Cs4 3.276(5) . ?
O2 Cs6 2.78(3) 1_554 ?
O2 Cs6 2.88(3) 2_656 ?
O2 Cs2 2.897(3) 2_656 ?
O2 Cs2 2.950(3) 1_554 ?
O2 Cs5 2.990(10) 2_656 ?
O2 Cs5 2.994(10) 8_454 ?
O2 Cs5 3.000(10) 1_554 ?
O2 Cs5 3.086(11) 7_656 ?
O2 Cs7 3.145(15) 7_656 ?
O2 Cs1 3.221(5) 8_454 ?
O3 Cs7 3.012(8) . ?
O3 Cs1 3.033(4) . ?
O3 Cs4 3.038(4) . ?
O3 Cs3 3.063(6) . ?
O3 Cs1 3.079(4) 2_757 ?
O3 Cs3 3.098(6) 2_757 ?
O3 Cs4 3.128(4) 2_757 ?
O3 Cs6 3.26(3) . ?
O3 Cs5 3.310(13) . ?
Cs1 Cs1 1.363(9) 2_757 ?
Cs1 Cs1 3.020(10) 7_657 ?
Cs1 Cs1 3.866(7) 8 ?
Cs1 Cs1 3.866(7) 8_455 ?
Cs2 Cs2 2.83150(9) 2_757 ?
Cs2 Cs2 2.83150(10) 2_657 ?
Cs3 Cs3 0.736(13) 6_565 ?
Cs3 Cs3 1.007(16) 2_757 ?
Cs3 Cs3 1.247(16) 5_767 ?
Cs4 Cs4 2.388(7) 2_757 ?
Cs4 Cs4 2.733(10) 6_565 ?
Cs4 Cs4 3.295(7) 2_657 ?
Cs4 Cs4 3.629(8) 5_767 ?
Cs5 Cs5 1.50(4) 7_657 ?
Cs5 Cs5 2.19(2) 2_757 ?
Cs5 Cs5 3.136(17) 8 ?
Cs5 Cs5 3.136(16) 8_455 ?
Cs5 Cs5 3.48(2) 2_657 ?
Cs6 Cs6 1.94(8) 2_657 ?
Cs6 Cs6 3.61(9) 6_565 ?
Cs6 Cs6 3.73(8) 2_757 ?
Cs6 Cs6 3.81(9) 7_657 ?
Cs7 Cs7 3.73(3) 7_657 ?
Cs7 Cs7 3.73(3) 7_757 ?
Cs8 Cs8 2.55(8) 5_767 ?
Cs8 Cs8 3.12(8) 5_667 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Te1 O2 Cu1 -0.001(1) 2_656 . . 7_656 ?
O3 Te1 O2 Cu1 -89.27(11) 2_656 . . 7_656 ?
O3 Te1 O2 Cu1 94.45(11) . . . 7_656 ?
O1 Te1 O2 Cu1 -178.22(12) 5_666 . . 7_656 ?
Te1 Te1 O2 Cu1 180.000(0) 5_666 . . 7_656 ?
Cs6 Te1 O2 Cu1 39.4(8) . . . 7_656 ?
Cs6 Te1 O2 Cu1 -135.7(8) 2_656 . . 7_656 ?
Cs4 Te1 O2 Cu1 53.74(14) . . . 7_656 ?
Cs4 Te1 O2 Cu1 -129.52(14) 2_656 . . 7_656 ?
O2 Te1 O2 Cs6 175.7(9) 2_656 . . 1_554 ?
O3 Te1 O2 Cs6 86.4(8) 2_656 . . 1_554 ?
O3 Te1 O2 Cs6 -89.8(8) . . . 1_554 ?
O1 Te1 O2 Cs6 -2.5(8) 5_666 . . 1_554 ?
Cu1 Te1 O2 Cs6 175.7(9) 7_656 . . 1_554 ?
Te1 Te1 O2 Cs6 -4.3(9) 5_666 . . 1_554 ?
Cs6 Te1 O2 Cs6 -144.9(16) . . . 1_554 ?
Cs6 Te1 O2 Cs6 40.0(15) 2_656 . . 1_554 ?
O2 Te1 O2 Cs6 135.7(8) 2_656 . . 2_656 ?
O3 Te1 O2 Cs6 46.5(8) 2_656 . . 2_656 ?
O3 Te1 O2 Cs6 -129.8(8) . . . 2_656 ?
O1 Te1 O2 Cs6 -42.5(8) 5_666 . . 2_656 ?
Cu1 Te1 O2 Cs6 135.7(8) 7_656 . . 2_656 ?
Te1 Te1 O2 Cs6 -44.3(8) 5_666 . . 2_656 ?
Cs6 Te1 O2 Cs6 175.1(8) . . . 2_656 ?
O2 Te1 O2 Cs2 102.88(16) 2_656 . . 2_656 ?
O3 Te1 O2 Cs2 13.61(14) 2_656 . . 2_656 ?
O3 Te1 O2 Cs2 -162.67(14) . . . 2_656 ?
O1 Te1 O2 Cs2 -75.34(16) 5_666 . . 2_656 ?
Cu1 Te1 O2 Cs2 102.88(16) 7_656 . . 2_656 ?
Te1 Te1 O2 Cs2 -77.12(16) 5_666 . . 2_656 ?
O2 Te1 O2 Cs2 -173.6(3) 2_656 . . 1_554 ?
O3 Te1 O2 Cs2 97.1(3) 2_656 . . 1_554 ?
O3 Te1 O2 Cs2 -79.1(3) . . . 1_554 ?
O1 Te1 O2 Cs2 8.2(3) 5_666 . . 1_554 ?
Cu1 Te1 O2 Cs2 -173.6(3) 7_656 . . 1_554 ?
Te1 Te1 O2 Cs2 6.4(3) 5_666 . . 1_554 ?
O2 Te1 O2 Cs5 109.3(3) 2_656 . . 2_656 ?
O3 Te1 O2 Cs5 20.0(3) 2_656 . . 2_656 ?
O3 Te1 O2 Cs5 -156.3(3) . . . 2_656 ?
O1 Te1 O2 Cs5 -69.0(3) 5_666 . . 2_656 ?
Cu1 Te1 O2 Cs5 109.3(3) 7_656 . . 2_656 ?
Te1 Te1 O2 Cs5 -70.7(3) 5_666 . . 2_656 ?
O2 Te1 O2 Cs5 94.1(4) 2_656 . . 8_454 ?
O3 Te1 O2 Cs5 4.9(4) 2_656 . . 8_454 ?
O3 Te1 O2 Cs5 -171.4(4) . . . 8_454 ?
O1 Te1 O2 Cs5 -84.1(4) 5_666 . . 8_454 ?
Cu1 Te1 O2 Cs5 94.1(4) 7_656 . . 8_454 ?
Te1 Te1 O2 Cs5 -85.9(4) 5_666 . . 8_454 ?
O2 Te1 O2 Cs5 -167.1(4) 2_656 . . 1_554 ?
O3 Te1 O2 Cs5 103.6(3) 2_656 . . 1_554 ?
O3 Te1 O2 Cs5 -72.6(3) . . . 1_554 ?
O1 Te1 O2 Cs5 14.7(3) 5_666 . . 1_554 ?
Cu1 Te1 O2 Cs5 -167.1(4) 7_656 . . 1_554 ?
Te1 Te1 O2 Cs5 12.9(4) 5_666 . . 1_554 ?
O2 Te1 O2 Cs5 171.6(9) 2_656 . . 7_656 ?
O3 Te1 O2 Cs5 82.3(9) 2_656 . . 7_656 ?
O3 Te1 O2 Cs5 -93.9(9) . . . 7_656 ?
O1 Te1 O2 Cs5 -6.6(9) 5_666 . . 7_656 ?
Cu1 Te1 O2 Cs5 171.6(9) 7_656 . . 7_656 ?
Te1 Te1 O2 Cs5 -8.4(9) 5_666 . . 7_656 ?
O2 Te1 O2 Cs7 98.1(9) 2_656 . . 7_656 ?
O3 Te1 O2 Cs7 8.8(9) 2_656 . . 7_656 ?
O3 Te1 O2 Cs7 -167.5(9) . . . 7_656 ?
O1 Te1 O2 Cs7 -80.1(9) 5_666 . . 7_656 ?
Cu1 Te1 O2 Cs7 98.1(9) 7_656 . . 7_656 ?
Te1 Te1 O2 Cs7 -81.9(9) 5_666 . . 7_656 ?
O2 Te1 O2 Cs1 83.5(3) 2_656 . . 8_454 ?
O3 Te1 O2 Cs1 -5.7(3) 2_656 . . 8_454 ?
O3 Te1 O2 Cs1 178.0(3) . . . 8_454 ?
O1 Te1 O2 Cs1 -94.7(3) 5_666 . . 8_454 ?
Cu1 Te1 O2 Cs1 83.5(3) 7_656 . . 8_454 ?
Te1 Te1 O2 Cs1 -96.5(3) 5_666 . . 8_454 ?
